advertisement

Applied Mathematical Modelling 37 (2013) 586–609 Contents lists available at SciVerse ScienceDirect Applied Mathematical Modelling journal homepage: www.elsevier.com/locate/apm FEM analysis for residual stress prediction in hot rolled steel strip during the run-out table cooling Xiaodong Wang a,⇑, Fei Li a, Quan Yang b, Anrui He b a b Shougang Research Institute of Technology, Shougang Group, No. 69 Yangzhuang Street, Shijingshan District, Beijing 100043, PR China University of Science and Technology Beijing, 30 Xueyuan Road, Haidian District, Beijing 100083, PR China a r t i c l e i n f o Article history: Received 11 May 2011 Received in revised form 9 February 2012 Accepted 29 February 2012 Available online 9 March 2012 Keywords: Hot rolled strip Internal stress Phase transformation Run-out table Flatness ABAQUS a b s t r a c t With the increasing demand of higher quality hot rolled strips, ﬂatness defects occurred on the strips during the cooling process on the run-out table have received signiﬁcant attention and should be considered in the online shape control model. Non-uniform temperature distribution and cooling across the strip width are the main reasons why the strip becomes unﬂatten after cooling process although the strip is rolled ﬂat at the ﬁnishing mill. A thermal, microstructural and mechanical coupling analysis model for predicting ﬂatness change of steel strip during the run-out table cooling process was established using ABAQUS Finite Element Software. In this model, Esaka phase transformation kinetics model was employed to calculate the phase transformation, and coupled with temperature calculation by means of the user subroutine program HETVAL. An elasto-plasticity constitutive model of the material, in which conventional elastic and plastic strains, thermal strain, phase transformation strain and transformation induced plastic strain were taken into account, was derived and realized using the user subroutine program UMAT. The conclusion that the ﬂatness of the steel strip will develop to edge wave defect under the functions of the different thermal and microstructural behaviors across strip width direction during the run-out table cooling procedure was acquired through the analysis results of this model. The calculation results of this analysis model agree with the actual measurements and observation, therefore this model has a high accuracy. To better control the ﬂatness quality of hot rolled steel strip, the shape compensation control strategy of slight center wave rolling is proposed based on the analysis result. This control strategy has been veriﬁed by actual measurements, and applied in actual production. Ó 2012 Elsevier Inc. All rights reserved. 1. Introduction After the steel strip is hot rolled, it is then subjected to cooling on the run-out table. The qualities of the ﬁnal product, such as the metallurgical and mechanical properties and the ﬂatness, may vary signiﬁcantly depending on the cooling process. The strip may show non-ﬂatness during the run-out table cooling because of the internal stress generated in it. The level of internal residual stress in hot rolled steel strip has recently been recognized as an important quality parameter [1]. If the residual stresses are not controlled or released, problems may arise in the following processing operations. For instance, the longitudinal cuts will be deformed. Quality complaints arise about the non-ﬂatness problems are due to the residual stress released when the steel sheets are cut to use. ⇑ Corresponding author. Tel.: +86 13681174531; fax: +86 10 88295026. E-mail address: [email protected] (X. Wang). 0307-904X/$ - see front matter Ó 2012 Elsevier Inc. All rights reserved. http://dx.doi.org/10.1016/j.apm.2012.02.042 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 587 With the increasing demand of higher quality hot rolled strips, ﬂatness defects occurred on the strip during the cooling process have been recognized and should be considered in the online shape control model. The evident unﬂatten or latent unﬂatten defects on the strip are caused by the residual stress due to uneven thermal and microstructural behaviors during the cooling. Large residual stress may cause local plastic deformation across the strip and consequently induce strip ﬂatness defect. Narrow bands will undergo serious distortions because the internal equilibrium of the residual stress ﬁeld is destroyed when steel strip is cut, even though the strip had no manifest shape defect before cutting. It is a complicated process for the strip cooling on the run-out table during which thermal stress will generate due to uneven cooling along the transverse direction. Other than the thermal stress, the uneven phase transformations also lead to internal stress generation in the strip. Both the thermal and transformation stresses are the sources of the residual stress leading to the ﬂatness defects. The residual stress must be controlled to be as low as possible in the actual production. Many researches [2–5] on the heat transfer and metallurgical phenomena during the cooling of hot rolled strip have been carried out. On the contrary, even though many mill engineers and researchers are keenly interested in precise prediction and control the residual stresses generated in the strip during the run-out table cooling, the researches on this aspect are still not adequate to solve the problem. Precise investigation of the residual stress developed in the strip during the cooling has become more and more important, and has received signiﬁcant attention [6–17]. Yoshida [6] proved that uniform transverse temperature distribution and even cooling can prevent wavy edges on the hot rolled steel strip after cooling, and also mentioned that higher coiling temperature is beneﬁcial to reduce the residual stress through a numerical temperature and thermal stress analysis. In the research of deﬂections of the thermomechanical controlled process (TMCP) plates conducted by Wang et al. [7], the temperature drop at strip edge will lead to center wave ﬂatness defect occurring at the ﬁrst deﬂection stage during or after cooling and before hot leveling, while it will lead to edge wave ﬂatness defect occurring at the second deﬂection stage during the ﬂattened plate is air cooled to ambient temperature. Yoshida et al. [8] developed a predictive mathematical simulator of temperature, thermal stress and shape defect during accelerated cooling in steel plate, and proved by longitudinal cutting test. Suzuki and Isaka [9] concluded that the temperature uniformity in plates is important to control the residual stress and improve ﬂatness accuracy of plates during hot levelling based on the FEM and the model testing results. Tani et al. [10] developed an on-line shape control system including buckling and camber estimation techniques and residual stress control technique by means of roller levelling for plate during cooling process. During the analysis it was proved that the shape defect will be the edge wave after the cooling because of the uneven temperature distribution. Cai [11] also acquired the conclusion in his thesis paper that the edge wave will happen after the cooling of steel strip even though the strip is ﬂat after the rolling. Han et al. [12] developed a two dimensional FEM model to simulate the deformation, temperature and phase transformation behavior in thickness and width direction of steel strip during run-out table cooling. Edge deformations of strip can be predicted while ﬂatness defects can not be acquired using this model. Colás et al. [13] developed a simple model to predict the wavy edge shape defects resulted by thermal and microstuctural gradients across the width of the strip during the cooling processes. A preliminary computational analysis of the residual stress generation during the cooling process of hot rolled thin gauge strip on the run-out table was performed by Zhou et al. [14]. While the conclusion is that the center wave happens on the strip after cooling. One consistent shape prediction simulator was developed by Ogai et al. [15], in which the cooling courses the run-out table, downcoiler and coil yard were covered. The calculation shows that center wave occurs on the strip during its cooling on the run-out table, and then center wave weakens during coiling in the downcoiler, in the end center wave disappears and edge wave appears during cooling at the coil yard. Zhou et al. [16] showed that temperature drop in the edge will result to wavy edges on the strip during the run-out table cooling. Nikitenko and Gris [17] also observed that ﬂatness deterioration can be caused by non-uniform water cooling across the strip width during strip transport through laminar cooling on the run-out table, which is a result of excessive thermal contraction in the over-cooled strip edges. The measure that lower coiling temperature can lead to phase transformation completion across strip width was put up forward to improve that situation. However, it seems unreasonable. The maximum residual stress in hot rolled steel strip measured by Hidveghy et al. [1] was about 115 MPa. However, the size of the sample was small with 250 mm both in the width and length, parts of the residual stresses may be released during the sample cutting. Modeling for precise prediction of the residual stresses in the steel strip during the cooling processes is a difﬁcult task due to the strong interaction among the thermal, mechanical and metallurgical behaviors, shown as in Fig. 1. In general, interactions 5 and 6, e.g. the inﬂuences of stress and strain on phase transformation and the temperature ﬁeld can be neglected in the modeling. In order to calculate the residual stress, the elastic strain, the plastic strain, the volumetric strain due to thermal and phase transformation, and the transformation induced plastic strain should be taken into account in the constitutive model. The inhomogeneous cooling and the difference of the phase transformation in the width direction of the strip on the run-out table give rise to the large residual stress. There is few work in which the effect magnitudes of the ﬁve sources of deformation mentioned above are reviewed in detailed up to now. Most of the researches [6–17] mainly focused on the thermal stress analysis with or without considering the phase transformation. The residual stresses calculated by Yoshida [6], Colás et al. [13] and Zhou et al. [14] are within the range of 50–100 MPa consisted of the volumetric changes due to the thermal and phase transformation. While in the research carried out by Cai [11] the residual stresses are 150–220 MPa although the phase transformation strain and thermal strain were taken into account. The transform induced plastic strain was considered as well as the thermal and phase transformation induced volumetric strains in the work of Han et al. [12]. The investigation results showed the elastic strain, plastic strain, phase transformation induced volumetric strain, and the 588 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 Fig. 1. The interactions among the thermal, mechanical and metallurgical behaviors. transformation induced plastic strain are 0%, 30%, 10% and 60% in total strain and the displacement will be signiﬁcantly underestimated when the transformation induced plastic strain is neglected. Yoshida et al. [8] conﬁrmed in their research that transformation has an important inﬂuence on prediction accuracy of the residual stress generation in the steel plate during cooling. Koo et al. [18] mentioned in their work the effect of transformation induced plasticity is required for precision analysis as a future work. The phase transformation induced plasticity (TRIP), which has an important inﬂuence on the residual stress ﬁeld during the metal heat treating, have been widely taken into account in the thermal, mechanical and metallurgical coupling analysis models [19–26]. TRIP, not a kind of normal plasticity behavior, can cause plastic ﬂow during the metallurgical phase transformation process although when the stress is much lower than yield stress limit of the material. The opening work explaining TRIP effect was carried out by Greenwood and Johnson. The constitutive model in which whether or not TRIP effect is considered is important for investigating temperature, phase transformation and stress-strain interactions during steel heat treatment [19–26]. Fischer et al. [22] brought forward a new view on TRIP, and presented a proposal for a modiﬁed constitutive law for elastic plastic phase changing materials. In the research of Yao et al. [24], the result veriﬁed that TRIP has a signiﬁcant inﬂuence on the ﬁnal stress distribution in the metal during heat treatment, for instance, at one point the residual stresses changes from 200 MPa when only thermal stress is considered to 30 MPa when the thermal and the phase volumetric strain are considered, and then to 70 MPa when the phase transformation induced plastic strain are taken into account additionally. Silva et al. [25] made the conclusion that great discrepancies will be introduced in the predicted residual stresses if phase transformation is neglected during the steel quenching. In the process of hot strip rolling, the steel strip on the run-out table is cooled down by mainly water as a kind of heat treatment, so it can be deduced that the phase transformations induced plasticity also have a great inﬂuence on the internal stress in the steel strip during the cooling process. However, this effect has not been emphasized in the early research works. Therefore, TRIP effect should be taken into account in the investigation of the residual stress generation in the steel strip during the cooling process. Wang et al. [27] analyzed the thermal stresses during the cooling of hot rolled strip on the run-out table using ﬁnite element method. Although phase transformations were considered in the model, both of transformation strain and transformation induced plastic strain have not been coupled with the thermal and stress behaviors. For a thorough investigation on how the strip ﬂatness changes during the cooling, a FE model in which temperature, phase transformation and stress/strain were fully coupled to analyze the internal stress evolution has been established using ABAQUS in this work, and the results were compared with the measurements. 2. Mathematic models used in FEM 2.1. Thermal model The thermo-mechanical analysis involves solving the transient heat transfer and thermal stress problem describing the temperature and thermal stress variations with time in the strip during cooling. During the run-out table cooling process, the temperature distribution in the strip can be calculated using the governing partial differential equation shown as follows: @ @T @ @T @ @T @T kx ðTÞ þ ky ðTÞ þ kz ðTÞ þ q_ ¼ qcp ðTÞ ; @x @x @y @y @z @z @t ð1Þ X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 589 where q is the density, cp(T) is the temperature dependent speciﬁc heat; k(T) is the temperature dependent thermal conductivity of the material with the subscripts x, y and z representing its components in three directions of width, length and thickness, respectively; T and t are temperature and time, respectively; and q_ is the rate of heat generation term representing the internal heat source released due to phase transformation of austenite q_ ¼ DHi DX i ; Dt ð2Þ where DHi is the amount of heat of transformation at temperature Ti and DXi is the transformed fraction within the time increment Dt. 2.2. Phase transformation model Hot rolled plain low carbon steel strip was selected as the research object. Esaka phase transformation dynamic model of plain C-Mn steel introduced in the reviewing paper of Kwon [28], was employed in this work. Esaka phase transformation dynamic model was established on the basic of Avrami function and is suitable to be applied in C-Mn steel. Two factors affecting k value namely austenite grain diameter Dc before phase transformation and retained strain De were considered, and the main structure of this model is as follows: 1 2:24 X ¼ X max 1 exp q þ 0:114ðDeÞ2 ð1 þ BðDeÞÞkðt sÞn ; 2:24 Dc ð3Þ where X and Xmax are the transformed fraction and the maximum fraction of one phase, respectively; t is the time; incubation period s and parameters k and n used in the phase transformations of austenite to ferrite, pearlite and bainite are respectively determined by Eqs. (4)–(6) expressed as follows: 8 > ln sF ¼ 1:6454 ln kF þ 20 ln T þ 3:265 104 T 1 173:89; > > > < k ¼ expð4:7766 13:339½%C 1:1922½%Mn þ 0:02505ðT 273Þ; F > 3:5607 105 ðT 273Þ2 Þ; > > > : nF ¼ 1:0; ð4Þ 8 4 1 > > > ln sP ¼ 0:91723 ln kP þ 20 ln T þ 1:9559 10 T 157:45; > < k ¼ expð10:164 16:002½%C 0:9797½%Mn P > þ0:0079ðT 273Þ 2:313 105 ðT 273Þ2 Þ; > > > : nP ¼ 1:0; ð5Þ 8 > ln sB ¼ 0:68352 ln kB þ 20 ln T þ 1:6491 104 T 1 155:30; > > > < k ¼ expð28:784 11:484½%C 1:112½%Mn B > þ0:13109ðT 273Þ 1:2077 104 ðT 273Þ2 Þ; > > > : nB ¼ 1:4; ð6Þ where T is the temperature; [%C] and [%Mn] are the weights of chemical C and Mn in percentage, respectively; subscripts A, F, P and B represent austenite, ferrite, pearlite, and bainite, respectively; the formulae for calculating parameter q used in the Eq. (3) is illustrated in [28]; parameter B is determined as 4 for ferrite and 100 for pearlite respectively; Xmax values related to the maximum ferrite fraction Fmax, pearlite fraction Pmax and Baintite fraction Bmax are determined as follows: X max 8 993K < T 6 Ar3 ; > < F max ¼ f ðTÞ ¼ Pmax ¼ f ð993Þ T PE < T 6 993K; > : Bmax ¼ 1 f ð993Þ T < T PE ; ð7Þ where the function f(T) is given as follows: f ðTÞ ¼ 1 ½%C=C 0 ; ð8Þ where C0 and TPE, are the carbon content in weight percentage at the temperature Ar3 and the transformation temperature of pearlite, respectively, C0 = 14.09 0.02973(T 273) + 1.5656 105(T 273)2. 2.3. Constitutive equations Total strain in steel strip can be decomposed into ﬁve parts due to different causes during the cooling procedure, and it can be written to be the incremental form [23] as follows dfeg ¼ dfege þ dfegth þ dfegp þ dfegtr þ dfegtp ; ð9Þ 590 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 where the symbols in {} hereinafter represent the vectors in this work; d{e}e, d{e}th and d{e}p are the increments of elastic strain, thermal strain and conventional plastic strain, respectively; d{e}tr and d{e}tp, relevant to phase transformation, are increments of phase transformation strain due to phase volume change and phase transformation induced plastic strain, respectively. Thermal strains due to non-uniform temperature distribution and cooling are depended on microstructural compositions: dfegth ¼ ðX A aA þ X F aF þ X P aP þ X B aB ÞT_ dij ; ð10Þ 1 i¼j is Kronecker tensor. 0 i–j Phase transformation strain increment due to phase volume change during the phase transformation process is calculated as follows: where a is thermal expansion coefﬁcient, °C1; dij ¼ dfegtr ¼ X ! ¼ 2I bk X_ k ð11Þ dij ; k where b is the phase transformation expansion coefﬁcient; subscripts 1, 2, and 3 represent austenite, ferrite, and pearlite, respectively; I is the total phase number. On the viewpoint of microstructure, TRIP effects usually can be explained through two mechanisms [29]: (1) Magee theory, ﬁtting to martensite transformation; (2) Greenwood–Johnson theory, ﬁtting to the situation mother phase will expansion because of new phase generation and then microstructural plastic strain is produced. Because there are only transformations from austenite to ferrite and pearlite in this research work, Greenwood-Johnson model was selected to describe the phase transformation induced plasticity. The phase transformation induced plasticity (TRIP) deduced by Greenwood and Johnson [19] is expressed as follows: etp ¼ 5 d r; 6 r0y ð12Þ where d is the strain due to phase volume change; r0y is the yield stress of mother phase. In Eq. (12), as well as in the subsequence, boldface letters and symbols represent the second-order tensors if there is no another special illustration. There are many researchers such as Abrassart, Leblond and Desalos who have modiﬁed the Greenwood–Johnson model, the model modiﬁed by Leblond is one of the most widely used in practical applications [23]: dfegtp ¼ 3 tp k uðXÞ X_ Sij ; 2 ð13Þ where ktp is the coefﬁcient of transformation induced plastic strain, a constant depended on the alloy contents of the steel; Sij is the deviatoric stress tensor; uðXÞ is a function of new phase volume fraction. To avoid the problem that Eq. (12) overestimates the transformation induced transformation plasticity at the beginning of transformation, Leblond proposed to disregard the transformation induced plasticity when the new generated phase fraction is less than or equal to 0.03. This conclusion has been veriﬁed to agree with reality through the results obtained by Taleb and Sidoro [29]. In this work, Leblond extended model was employed as the calculating formulation of TRIP composition of the material constitutive equation, and is expressed as follows: ( detp ij ¼ 0 eq 2Drey12 lnðXÞ X_ 32 hðrry Þ Sij if X 6 0:03 ; if X > 0:03 ð14Þ A where De12 is the volume change due to austenite transforms to thenew phase; ryA is the yield stress of austenite; ry is the eq yield stress of the mixed structure; req is the equivalent stress; h rry is the nonlinear term when the exerted stress is more y than half of r : ( eq 1 if rry 6 12 req ¼ h eq y r 1 þ 3:5ðrry 12Þ if req ry > 12 ; ð15Þ Derivation work on the material constitutive equations can be divided into two segments, namely elastic and plastic deformations. At beginning of each step during the calculation, whether phase transformation has started or not will be judged. If the phase transformation occurs and its volume fraction is larger than 0.03, according to Eq. (14), transformation induced plastic ﬂow happens even though the equivalent stress is lower than the yield stress. Transformation plastic strain ﬂows along the direction of the current derivatoric stress. Constitutive function when transformation induced plastic behavior happens can be expressed as follows [24]: dfrg ¼ ½Dtp dfeg df~egth dfegtr ; ð16Þ 1 ½Dtp ¼ K1 1 þ 2Gg0 I 1 1 2Gc0 n n; 3 ð17Þ where X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 E ðTÞ 591 E ðTÞ K ¼ 3ð12p v p ðTÞÞ and G ¼ 2ð1þpv p ðTÞÞ are bulk and shear modules, respectively; 1 and I are the second order and the fourth order identity tensors, respectively; g0 and c0 can be calculated according to the formulae in [24]. In the elastic deformation region, the total strain increment can be expressed as follows: dfeg ¼ dfege þ dfegth þ dfegtr þ dfegtp : ð18Þ The elastic strain is linearly related to the applied stress by isotropic Hooke’s law, and then stress increment rij can be derived and expressed as the vector form in which material properties parameters depended on temperature are considered dfrg ¼ ½Del ðdfeg df~egth dfegtr dfegtp Þ; ð19Þ where " # d½D1 el _ df~eg ¼ ðX A aA þ X F aF þ X P aP þ X B aB Þ½ 1 1 1 0 0 0 þ frg T; dT th T ð20Þ where [D]el can be described as the tensor form: Del ¼ K1 1 þ 2G½I ð1=3Þ1 1: ð21Þ When the material undergoes macro plastic deformation, the total strain increment can be expressed as follows: dfeg ¼ dfege þ dfegth þ dfegp þ dfegtr þ dfegtp : ð22Þ Based on the relationship between elastic stress and elastic strain, stress increment can be rewritten as follows: dfrg ¼ ½Del ðdfeg dfegp df~egth dfegtr dfegtp Þ: ð23Þ To the metal plastic material such as steel, plastic strain increment is related to the yield facet. In this work, isotropic hardening Von-Mises yield criterion and Prandtl–Reuss plastic ﬂow rule were employed: f ðrij Þ depij ¼ 1 2 r ¼ 0; 3 s0 3 p de nij ; 2 ð24Þ ð25Þ p ; dep the equivalent plastic strain rate, whereqrﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ the plastic strain rate; nij ¼ Sij =r s0 is the yield stress of material; deij q ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ the equivalent stress, r ¼ 32 Sij Sij . dep ¼ 3=2depij depij ; r R dep : Assume H is the rate of slope at any one point of hardening curve r H¼ dr : dep ð26Þ Through derivation, the constitutive equation (23) when the material undergoes plastic deformation was expressed as follows: dfrg ¼ ½Dep ðdfeg df~egth dfegtr dfegtp Þ; ð27Þ T ½Del @[email protected] g @[email protected] g ½Del ½Dep ¼ ½Del : T H þ @[email protected] rr g ½Del @[email protected] g ð28Þ where 3. FEM analysis model This numerical analysis work was carried out on the basic of the real production processes and conditions in one hot strip mill in Shougang Group. The run-out table is 130 m long and the behavior of a strip with a certain length was investigated. A fully coupled temperature-displacement analysis of the internal stress in the strip developed during cooling was carried out using ABAQUS Version 6.5 [30], which provides the pre- and post- processors and the solvers for the ﬁnite element analysis. That software provides the user with many user subroutines as powerful tools to accurately simulate the non-linear boundary conditions, loads, and constitutive behavior of materials. A ﬁnite element model of the strip cooling process covering the full length of the run-out table will be computationally inefﬁcient and high cost. One segment of the strip with 6 m length was chosen to be the research object. During the cooling process, the strip is transported on the run-out table, while the cooling proﬁle is stationary in time. For convenience of calculation, it is assumed that the cooling process is moving with a static strip. The steel grade of the strip selected to be calculation object is HP295. 592 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 3.1. Meshing of the physical model The length, width and thickness of the strip segment to be computed are 6 m, 1200 mm and 4.0 mm, respectively. Strip velocity was assumed to be 6.0 m/s. The strip is cooled from 880 to 620 °C on the run-out table. The model was established in the rectangular coordinate system, and the directions 1, 2 and 3 represent width, thickness, and length respectively. Element type is C3D8T, and element size is 30 mm. Meshes of the computation model is shown in Fig. 2. 3.2. Determination of the physical parameters The material physical parameters depending on temperature have important effects on the results of computation. It is necessary to correctly select the physical parameters for ensuring the computation precision of the temperature and internal stress. Low carbon steel HP295 was selected as the computation subject, material characteristic parameters such as speciﬁc heat, thermal conductivity coefﬁcient were provided by hot strip mill of Qiangang Iron and Steel Company of Shougang Group as shown in Table. 1. Young’s modulus and Poisson’s ratio, hardening curves, which were determined according to Ref. [14] as shown in Figs. 3 and 4, were deﬁned in the input ﬁle and passed into the user subroutine program UMAT of material constitutive model. Other material characteristic parameters including density, yield stress of every phase are shown as in Fig. 5, and thermal and phase expansion coefﬁcients are given in Eq. (29) and Eq. (30), respectively. They are all depended on the temperature, and directly deﬁned in the user subroutine program UMAT. The linear mixed rule was employed to calculate the parameters on the given temperature points, and then the value located between two temperature points was obtained by the linear interpolation method. Thermal expansion coefﬁcient (106 °C1) of each phase is determined as follows [11]: 8 3 > < aA ¼ 16:4 þ 6:6 10 T aF ¼ 12:34 þ 3:58 103 T ; > : aP ¼ 15:5 ð29Þ Phase expansion coefﬁcient is given by Cai [11] ( bA!F ¼ 2:17 103 þ ½ð750 TÞ 4:06 þ ð7502 T 2 Þ 1:51 103 106 ; bA!P ¼ 4:81 103 þ ½ð700 TÞ 0:9 þ ð7002 T 2 Þ 3:3 103 106 : ð30Þ 3.3. Boundary conditions To solve the temperature differential equation, it is very important to deﬁne boundary conditions accurately. The laminar cooling of the hot rolled strip on the run-out table is a relatively complicated process of heat transfer. The boundary conditions can be generalized to be convection heat transfer equation between the strip surface and cooling water and the radiative equation between the strip and the atmosphere. The boundary conditions can be described as follows Fig. 2. Meshes of the computation model. 593 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 Table 1 Thermal conductivity coefﬁcient and speciﬁc heat depended on temperature. Temperature °C Thermal conductivity coefﬁcient W/(m K) Speciﬁc heat J/(kg K) 550 600 650 700 750 800 850 900 950 34.4 31.8 28.5 27.2 26.2 25.8 25.5 25.4 25.5 692 735 752 866 1021 839 742 725 718 2.10E+11 0.35 0.34 1.90E+11 0.32 1.50E+11 0.31 1.30E+11 0.3 1.10E+11 0.29 E u 9.00E+10 0.28 Poisson's ratio Young's modulus /Pa 0.33 1.70E+11 0.27 7.00E+10 5.00E+10 0.26 0.25 0 100 200 400 450 500 550 600 650 675 700 725 750 775 800 825 850 875 Temperature / Fig. 3. Young’s modulus and Poisson’s ratio depended on temperature. 5.00E+08 4.50E+08 True stress /Pa 4.00E+08 3.50E+08 3.00E+08 2.50E+08 2.00E+08 1.50E+08 1.00E+08 T=0 T=200 T=280 T=400 T=600 T=750 T=800 T=1000 5.00E+07 0.00E+00 0 0.05 0.1 0.15 0.2 0.25 0.3 0.35 True strain Fig. 4. Plastic characteristic curves depended on temperature. 0.4 0.45 0.5 594 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 Fig. 5. The yield stress of every solid phase [31]. ( k @T ¼ hw1 ðT T w1 Þ; @n k @T ¼ hw2 ðT T w2 Þ þ reðT 4 T 4w2 Þ; @n ð31Þ where n is normal direction of strip’s surface; hw1 and hw2 are convection heat transfer coefﬁcients on the strip surface between the cooling water and the air, respectively; r is Stefan–Boltzmann constant, 5.6697 108 W m2 K4; e is emissivity and setup to be 0.7 in this model; Tw1 and Tw2 are temperatures of cooling water and atmosphere, respectively. Just after the exit of the last ﬁnishing stand, there exists a length of about 10m where the strip is cooled in air, called air cooling zone. Following this region, the strip enters into water cooling zone. A certain rows of water jets impinge on the strip surface to take away the heat in the strip. From the last bank of water cooling to the coiler, there also exits an air cooling zone. Forced convection heat transfer and stable ﬁlm boiling respectively take place in two water ﬂowing zones of impinging zone and parallel ﬂowing zone on the strip surface. Too much computation time is needed to deﬁne the two kinds of heat transfer conditions very close to reality. Therefore, to make analysis simple, the total length of the run-out table has been divided into two different kinds of cooling zones, namely water cooling and air cooling. The water cooling zone is treated as a whole part, and one average heat ﬂux referred to Cox et al. [32] is assumed during the analysis. The heat ﬂux value can be adjusted to represent the running speed of the strip, and described in the following analysis. The detailed structure of the run-out table and thermal boundary conditions can be seen in Fig. 6. Mechanical boundary conditions also should be deﬁned during the internal stress analysis of the strip cooled on the runout table after hot rolling. Boundary Constraint conditions are deﬁned during the establishment of FEM model using the ABAQUS. Full displacement constraint is applied to one end of the strip segment, while the other end is assumed to be free. Two strip edges are assumed to be simply support condition along y direction normal to the rolling direction. 3.4. Initial conditions When steel strip leaves the last stand of ﬁnishing mill and before it enters into cooling zone, one initial temperature ﬁeld and one initial stress distribution already exist. Both of the initial temperature ﬁeld and initial stress are not uniform. ABAQUS software provides user subroutine programs to realize uneven ﬁeld variables loading. Actual temperature measurements along transverse direction on the strip were carried out by means of two infrared thermal imagers at the exit of last stand of ﬁnishing mill and the entry of the downcoiler. Transverse temperature distribution can be ﬁtted to a fourth order polynomial function of transverse coordinate using the least squares method. By means of user subroutine program UTEMP, initial temperature ﬁeld as shown in Fig. 7 was deﬁned. Because the thickness of strip to be analyzed is very thin, uniform initial temperature distribution through the thickness direction of strip was assumed in the analysis. The result of initial temperature ﬁeld loaded on the analysis model can be seen in Fig. 8. After ﬁnish rolling, a stress distribution representing a certain ﬂatness pattern already exists in the strip. To simulate the initial ﬂatness, initial stress distribution should be loaded. The initial stress distribution can be expressed using relative X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 595 Fig. 6. (a) Structure of run-out table cooling; (b) thermal boundary conditions for water cooling and air cooling. Fig. 7. Initial temperature distribution along transverse direction of strip. elongation difference along transverse direction of the strip. As shown in Fig. 9, ez (x), x coordinate and z coordinate represent the relative elongation difference between center and edge of strip, width and length directions of strip, respectively. Initial stress can be determined as follows: 596 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 Fig. 8. Initial temperature ﬁeld of the strip loaded through UTEMP. rz ðxÞ ¼ Eez ðxÞ ¼ Eðepm epz ðxÞÞ; ð32Þ where E is Young’s modulus of material with end rolling temperature, MPa; epz (x) is the elongation of ﬁber at x coordinate, m; epm is the mean elongation of strip along transverse direction, and can be calculated by the following equation. epm ¼ Rb b epz ðxÞdx 2b ; ð33Þ where b is one half width of the strip, m. Based on the large amount of actual ﬂatness gauge measurements, epz (x) is assumed to be a parabolic curve epz ðxÞ ¼ a0 þ a1 x þ a2 x2 ; Fig. 9. Relationship between initial ﬂatness and internal stress (a) edge wave (b) center buckle. ð34Þ X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 597 where a0, a1, and a3 are coefﬁcients of the function which are determined according to the initial ﬂatness I Unit distribution. Same as the initial temperature, initial stress was loaded by means of the user subroutine program SIGINI, and the result of initial stress is shown as in Fig. 10. As two initial parameters in the phase transformation calculation, the austenite grain size and retained strain also need to be deﬁned. According to the research result obtained by Zhang et al. [33] that the austenite grain diameter after hot rolling and before the cooling is within the range of 20–40 um. The steel chemical compositions and the processing parameters in Ref. [33] are similar to those in this work. Therefore the austenite grain diameter Dc is assumed to be 20 um. Retained strain De in the strip after ﬁnish rolling is calculated as follows De ¼ ðfD ec þ fN eÞ expð1 ðt=st Þk Þ; ð35Þ where fD and fN are the volume fractions of dynamic recrystallization and non-recrystallization, respectively, determined by Esaka calculation models seen in Ref. [28]; ec is the deformation value when recrystallization begins; R is the gas constant; st = 8.46 109exp(43800/RT); e is the total deformation from reduction as deﬁned below 2 e ¼ pﬃﬃﬃ lnð1 PÞ; ð36Þ 3 where P = (H h)/H is the reduction of thickness, H and h are the thickness values before and after the deformation process respectively. 4. Results and discussion In this work, HP295 steel grade produced in one hot strip mill of Qiangang Iron and Steel Company of Shougang Group was selected as the research object, and the chemical compositions are shown in Table. 2. Computation procedure in the FEM model is divided into three steps. (1) The ﬁrst step is air cooling process of 12.7 m distance from the last stand ﬁnishing mill F6 to the ﬁrst row of laminar water cooling pipes. Air temperature and its convective coefﬁcient were assumed to be 30 °C and 30 W m2 k1, respectively. (2) The second work step is water cooling process lasting 10 s, heat ﬂux values on strip top surface and bottom surface were set to be 2.4 107 and 1.8 107 W m2, respectively. The atmosphere temperature was 28 °C. (3) The third work step is also air cooling and the time is 4 s. The related parameters for boundary conditions are same as those of the ﬁrst work step. 4.1. Realization of the thermal, metallurgical and mechanical coupling analysis ABAQUS Finite Element Software has been widely applied in the numerical simulations of many industrial processes such as metal plastic forming and heat treatment. In this study, ABAQUS was employed to realize the coupling analysis of the thermal, metallurgical and mechanical behaviours to calculate the internal stress evolution during the strip cooling process. Fig. 10. One example of initial stress in strip, 20 I Unit ﬂatness. 598 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 Table 2 Chemical composition of steel HP295 used in simulation (in wt%). C Si Mn P S Al 0.174 0.014 0.9 0.011 0.009 0.02 Esaka phase transformation model described in Item 2.2 was employed to calculate the microstructural evolution, and it was programmed in the user subroutine program HETVAL. Both of the transformation phase fractions and latent heat were calculated, as a results coupling between the phase transformation and temperature ﬁeld was realized. Other important parameters such as phase fractions, phase increments, incubation time of phase transformation, beginning transformation temperature, initial residual strain and austenite grain diameter, and so on were deﬁned as the state variables and initialized in the user subroutine program SDVINI. 51 state variables were deﬁned and the detailed is introduced as follows: STATEV(1) to STATEV(5) represent the fractions of austenite, ferrite, pearlite, bainite and martensite, respectively; STATEV(6) to STATEV(8) represent the incubation time of ferrite, pearlite and bainite, respectively; STATEV(9) to STATEV(12) represent the fraction increments of ferrite, pearlite, bainite and martensite, respectively; STATEV(13) and STATEV(14) represent the initial grain size of austenite and the residual strain, respectively; STATEV(15) to STATEV(20) represent the six components of elastic strain, respectively; STATEV(21) to STATEV(26) represent the six components of plastic strain, respectively; STATEV(27) represents the equivalent plastic strain; STATEV(28) to STATEV(33) represent the six components of phase transformation induced plastic strain, respectively; STATEV(34) to STATEV(39) represent the six components of thermal strain, respectively; STATEV(40) to STATEV(45) represent the six components of phase transformation strain, respectively; STATEV(46) to STATEV(48) represent the phase equilibrium temperatures of ferrite, pearlite and bainite, respectively; STATEV(49) to STATEV(51) represent the beginning temperatures of phase transformation for ferrite, pearlite and bainite, respectively. These state variables were updated in the calculation processes of HETVAL and UMAT. The material constitutive model introduced in Item 2.3 was programmed in the user subroutine program UMAT. The ﬂow charts of subroutines HETVAL and UMAT are shown as Figs. 11 and 12, respectively. Full coupled analysis of the thermal, mechanical and microstructural behaviors was realized by means of these subroutines with the help of these state variables. 4.2. Temperature and phase transformation calculation results To clearly analyze the inﬂuences of cooling process on the ﬂatness of the strip and to provide the initial temperature data and to verify the FEM model, the temperature distributions along strip width at the exit of the ﬁnishing mill and the entry of the downcoiler were measured by means of two infrared thermal imagers at the same time. The strip information such as coil number, steel grade, gauge, end rolling temperature and coiling temperature were recorded. Large amount of measurements were conducted and recorded, and then processed, one example is shown in Fig. 13. Precision of the temperature computation is the foundation of the internal stress analysis. To prove consistency of the calculation result of temperature with the production data, ﬁnish rolling temperature and coiling temperature recorded by system can be used. During the actual production, only the temperature at the steel strip center is measured and controlled. The calculation result of temperature evolution along strip’s transverse direction during the run-out table cooling is shown in Fig. 14. The temperature on the strip center at the exit of ﬁnish rolling mill is 880 °C, while about 620 °C after the cooling. Temperature evolution calculation result is of consistency with the temperature control requirement of the steel grade HP295 in the actual production. The temperature proﬁle along the strip width can be extracted from the measurement result of the infrared thermal imager. The temperature distribution comparison between the actual measurement and the calculation at the coiling stage is shown as in Fig. 15. It is mentioned before the temperature proﬁle measurement at the exit of the ﬁnishing mill was input into the model as an initial temperature condition. We can deduce that there is a well agreement between the FEM analysis and the measurement. As a result, it shows that the temperature calculation of this analysis model has a high accuracy. We can say that the thermal boundary conditions were correctly determined in this model. The strip has a non-uniform temperature distribution along its transverse direction with a certain temperature drop in the edge region, and this non-uniform distribution of the temperature retains until the end of the run-out table cooling. The phase transformations from austenite to ferrite and pearlite take place during the run-out table cooling. At the beginning of water cooling, temperature decreases with a high speed, while this trend becomes not so much at the later period of water cooling because of the latent heat released by the phase transformations. It is well known that temperature plays a great role in the phase transformation in the steel. The non-uniform distribution of temperature is the main reason for the uneven phase transformation in the strip. For the steel grade calculated, there are mainly the transformations of austenite to ferrite and pearlite in the steel during the run-out table cooling, and the end microstructure is also consisted of ferrite and pearlite. The phase fraction distribution calculation results of austenite, ferrite X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 599 Fig. 11. The calculation ﬂow chart of the subroutine program HETVAL. and pearlite along strip’s transverse direction were extracted from the model and can be seen as shown in Figs. 16–18, respectively. Uneven phase transformation process existing along the transverse direction of steel strip can be observed. Because the main inﬂuence factors on the phase transformation are the temperature and the cooling rate, in turn the uneven phase transformation is caused by non-uniform temperature distribution. Phase transformation happens ﬁrstly at the edge region of steel strip because of the temperature drop. Fig. 19 is the calculation results of phase transformation dependent on temperature at the center and edge of the strip. The temperature trajectories on the center and edge can also be seen as shown in Fig. 19. The temperature difference between center and edge is large at the beginning of cooling process, and then becomes small at the end of cooling process. The phase transformation behaviors occur mainly during the water cooling process, the incubation time is very short. At the end of the cooling, all austenite transform to ferrite and pearlite, and the microstructure fraction difference between the center and edge also is shown in Fig. 19. To verify the phase transformation calculation results, quantitative microstructure measurements were carried out. Seven samples of hot rolled steel strip HP295 with 1200 mm in width and 4.0 mm in thickness were cut. Microstructure measurements were made at nine positions evenly located along the transverse direction on every sample. All samples were ground and polished, and etched using 4% natal liquid, then microstructure were observed and photographed under the optical microscope DMIRM. The average of the measurement results at the same width point for seven samples was conducted, and the measurement and calculation results of the microstructures are shown as in Fig. 20. Ferrite fraction reaches as high as about 95% at the edge part of strip and as low as about 80% at the center part of strip, on the contrary pearlite fraction is about 20% and 5% at center and edge parts, respectively. Statistical analysis was carried out to compare between the measurement and calculation results of ferrite and pearlite phase fractions. The standard error of the calculation results to the measurements is 0.065 for both of ferrite and pearlite. The ratio of the standard error to the average fraction has a lower level 600 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 Fig. 12. The calculation ﬂow chart of the subroutine program UMAT. for ferrite with 6.8% at the edge part and 7.9% at the central part. But for pearlite, this standard error level is large because the fraction of pearlite is small. The ratio of the standard error to the average fraction is 119% at the edge part and 37% at the central part. It is very difﬁcult to predict the phase transformation precisely during the cooling process of the steel strip. Consequently we can deduce that the calculated results of phase fractions along transverse direction of strip agree with the measurement conducted on the end product as a reasonable accuracy. The phase transformation model adopted in this work can predict the microstructure evolution in this kind of steel strip during the cooling with a satisﬁed precision. From the temperature and microstructure analysis, it can be concluded that the non-uniform temperature distribution will lead to uneven microstructure evolution in the steel strip during the cooling process. And then, these inhomogeneous behaviors in steel strip will result with internal stresses and have great inﬂuences on the strip ﬂatness. 4.3. Stress analysis results Because the transverse and normal stresses in steel strip are very small and the strip ﬂatness is mainly attributed by longitudinal stress distribution along transverse direction, only longitudinal stresses are considered in this work. Fig. 21 is the X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 601 Fig. 13. One example of thermal image result and related processed data. longitudinal stress distributions along transverse direction at different cooling stages without initial stress and phase transformation. The thermal stress in the strip increases as the temperature of strip decreases rapidly after the strip enters into 602 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 Fig. 14. Temperature evolution along strip’s transverse direction. Fig. 15. Temperature distribution along the width of the strip at the coiling stage. water cooling zone. During air cooling, thermal stress increases slowly. The reasons for thermal stress generation are uneven temperature distribution and a high cooling rate. The compressive stress at the strip edge region reaches almost 80 MPa, and mainly concentrates within the range of 120 mm to the strip edge. For making a comparison between the results obtained in this work and those of the Refs. [6,11,14], the summary of analysis results of typical references was conducted and listed in Table. 3, in which mainly the steel grades, gauges, stress results and boundary conditions were concerned. The steel grade and the working conditions researched in this work have some differences with those in these references. However, the qualitative comparison can be made. The pattern of the longitudinal stress distribution agrees well with that obtained by Yoshida [6] and Cai [11], but is opposite to that of Zhou et al. [14]. There generates compressive stress in the strip edge region within 200 mm while tensile stress in the center part. The temperature drop at the strip edge region and the non-uniform cooling will lead to edge wave ﬂatness defect. The magnitude order of the stress is close to that of Zhou et al. [14] and Yoshida [6], while is much lesser than Cai’s result [11]. Temperature decrease within strip edge leads to the thermal stress distribution pattern of tensile stress at strip center region and compressive stress at strip edge region. That is to say, the strip ﬂatness may develop to edge wave under the function of the thermal stresses if there is a temperature drop at the strip edge region. In this part, phase transformation and initial stress were considered to analyze the internal stress evolution in the strip. Two working conditions of no initial stress and initial stress distribution of 10 I Unit ﬂatness were taken into account. The calculated results of the stresses can be seen as shown in Fig. 22. From the comparison between Figs. 22 and 21, we can know that the phase transformation behavior has a great inﬂuence on the internal stress. The largest compressive stress at the strip X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 Fig. 16. Austenite fraction distribution along strip’s transverse direction. Fig. 17. Ferrite fraction distribution along strip’s transverse direction. Fig. 18. Pearlite fraction distribution along strip’s transverse direction. 603 604 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 Fig. 19. Phase transformation and temperature trajectories at the center and edge of strip. Fig. 20. Microstructure measurement along transverse direction of strip. Fig. 21. Longitudinal tress distribution along transverse direction, in which initial stress, coiling tension and phase transformation were not considered. Table 3 The summary of analysis results of typical references. Steel gauges and chemical composition Temperature conditions Boundary conditions Cooling patterns Stress and shape results Yoshida [6] 3.24(thickness) 2173 mm(width); Fishing temperature: 880 °C; Heat transfer coefﬁcient H: (kcal/m2 h °C) Uniform and non-uniform cooling, early cooling and later cooling 0.14%C, 0.9%Mn, 0.05%Si Coiling temperature: 500–600 °C; 50–100 MPa compressive stresses at edge and 0–10 MPa tensile stresses at center Temperature drop at strip edge and non-uniform cooling lead to edge wave Uniform temperature and cooling, and high coiling temperature beneﬁt for shape Non-uniform early cooling Edge waves, compressive stresses of 150–250 MPa within the strip edge zone Uniform cooling, early cooling, later cooling and split cooling Central buckles, tensile stresses of 20–80 MPa at the region of 90 mm to strip edge, and compressive stresses of 5 MPa in the center Temperature difference: 46–109 °C H¼ Hrad þ Hconv ðair coolingÞ Hrad þ Hw ðwater coolingÞ Hrad ¼ em C s ½ðT s þ 273Þ2 þ ðT atm þ 273Þ2 ðT s þ T atm þ 546Þ c Hw ð1 þ 0:1ðB 10xÞ=BÞif x < 0:1B Hcw if x P 0:1B Hw ¼ 0:4 Hcw ðlower surfaceÞ 1100 early cooling Hw ¼ 1200 latter cooling em = 0.7–0.8; Cs = 4.88 105; Hconv = 7.5; B: width Same with those of Yoshida [6] Hw ¼ Cai [11] Zhou et al. [14] 3.0(thickness) 1560 mm(width); 0.14%C, 0.65%Mn, 0.18%Si 2.0(thickness)⁄1200mm (width);Chemical compositions are not available Fishing temperature: 900 °C; Coiling temperature: 600 °C; Temperature difference: 90 °C Fishing temperature: 860 °C; Coiling temperature: 540 °C; Temperature difference: 64–130 °C No detailed thermal boundary condition was given. The histories of the temperature proﬁles in both longitudinal and transverse directions were predetermined. X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 Reference 605 606 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 Fig. 22. Calculated and measured results of longitudinal stress distribution along strip’s transverse direction, phase transformation was considered. Fig. 23. Onsite observation of edge buckles on strip, (a) after cooling and before downcoiler, (b) uncoiling process. edge can reach to about 180 MPa when the effects of phase transformation induced strains are included in the material constitutive model. In the center part of the strip, the tensile stress also has an increase of about 20 MPa. The range of strip edge bearing compressive stress also extends from 120 mm when only the thermal stress is taken into account to nearly 200 mm. This illustrates that the stress generated due to the phase transformation is large and even bigger than the thermal stress. It can be deduced that the prediction result of edge wave defect with considering the phase transformation induced strains will be larger than that when only thermal stress is considered. The research work of a two deformation analysis model carried out by Han et al. [12] showed that the displacement in the thickness direction of steel strip is about 0.13 mm when TRIP effect is taken into account in the constitutive model vice verse it is only 0.02 mm when TRIP effect is not included. The displacement will be signiﬁcantly underestimated when TRIP effect is neglected. Without considering the TRIP effect on the internal stress, it is obvious that the calculation results obtained by Yoshida [6] and Zhou et al. [14] are somewhat underestimated while the results of Cai [11] are overestimated. Besides comparison with the results of references, for verifying this analysis model directly, residual stress measurements on the steel strip were also carried out. X-ray diffraction was adopted as stress measuring method, and the detailed measurements of residual stress also can be seen in Fig. 22. Two HP295 strip samples with length in 4.5 m, width in 1200 mm, and thickness in 4.0 mm were cut at the position nearly 15 m to strip coil heads. Because stress is much larger at strip edge than that at strip center, more measuring points were selected at the strip edge region. Flatness values of samples were recorded by the ﬂatness gauge at the exit of the ﬁnish rolling mill, and the detailed information is: there were 10 I Unit and 10 I Unit ﬂatness values within the heads of 50 m in the strip coil 6331401410 and 6331401380, respectively. There is a well agreement between the measurements and the calculations not only on stress distribution pattern but also on the magnitude level. It can be deduced that this analysis model has a high accuracy. It is also veriﬁed that the phase transformation has an important inﬂuence on prediction accuracy of the residual stress generation and the effect of transformation induced plasticity should not be neglected for precision analysis on the deformation of the steel plate during the cooling. X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 607 Fig. 24. Deformation of strip after cooling without initial stress. Fig. 25. Deformation of strip after cooling with initial stress of 10 I Unit ﬂatness. In accordance with the analysis results mentioned above, we can deduce that strip shape will develop to the trend of edge wave, and this phenomenon has been observed during the actual production as shown in Fig. 23. Strip shape after the ﬁnish rolling, namely the initial stress distribution in steel, has no inﬂuence on this trend. Initial stress only affects the magnitude of ﬁnal residual stress [27]. If the direction of initial stress is opposite to the direction of internal stress generated in the strip during the cooling process, then the residual stress will decrease, and inversely the residual stress will increase. That is to say the internal stress will decrease during the run-out table cooling process when the strip is rolled with a certain center buckles, and then the adverse inﬂuence of the cooling process on the strip shape can be reduced. Figs. 24 and 25 are the deformation results of the strip after cooling without initial stress and with the initial stress of 10 I Unit center buckle, respectively. When there is no initial stress loaded, the ﬁbers at strip edge have longer elongation than those at strip center as shown in Fig. 24. Then the strip shape will develop to the edge wave. When there is an initial stress distribution of 10 I Unit center buckle at beginning of cooling, the elongation difference between the edge and center becomes not so much after cooling as shown in Fig. 25. In the numerical analysis of the ﬂatness of thin strip conducted by Zhou et al. [16], it is showed that the buckling on the steel strip changes from the centre to the edge as the maximum difference in temperature between the edge and centre increases, correspondingly the edge wave becomes more severe during the cooling process on the run-out table. For the strip with 2 mm in thickness, the temperature drops of 100 °C and 130 °C between the edge and centre can lead to the edge buckles of 1026 I Unit and 64110 I Unit, respectively. The strip gauge researched 608 X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 Table 4 Measurements of actual ﬂatness values of steel strips. Coil no. Gauges (thickness width, mm) Steel grade Aim ﬂatness value setup at exit of ﬁnishing mill (I Unit) Actual ﬂatness value rolled at exit of ﬁnishing mill (I Unit) Position 5473V06030 5473V02010 5473V03030 5473V06360 5473V04040 5473V06350 5473V04030 5473R01010 5473M01010 5473V03010 2.73 1265 5.0 1250 3.98 1250 2.75 1250 2.75 1250 2.75 1250 2.75 1250 2.75 1250 5.48 1250 2.75 1250 Q235B Q235B Q235B Q235B Q235B Q235B Q235B SPCC Q235B Q235B 20 10 10 20 20 0 0 0 0 0 16 20 15 8 10 20 5 10 0 0 Strip Strip Strip Strip Strip Strip Strip Strip head head head head head head head head Flatness value measured during decoiling (I Unit) 30 m 40 m 60 m 30 m 30 m 50 m 40 m 40 m Flat Flat Flat Flat Flat 24 10 13 5 6 by Zhou et al. [16] is very thin and easier to be buckling at the same residual stress condition. The analysis result in this work has a good agreement with this kind of buckling trend. 4.4. Strip shape compensation control strategy From the analysis results presented early, the ﬂatness of hot rolled steel strip has a developing trend to edge wave during the run-out table cooling under the function of the temperature drop in the edge regions of the strip. Conventional measures to solve this problem try to improve temperature distribution uniformity along transverse direction through controlling water ﬂow rate distribution or edge masking [18,34]. However, those measures need modify and install new devices and control systems. That will increase the investing cost and affect normal production. The analysis results in this work show that the residual stress will decrease during the cooling process if the central buckle were rolled on the strip before cooling. As a result, one shape compensation control strategy of slight central wave rolling is proposed in this work. The main idea is that steel strip is rolled with a certain slight center buckle at the exit of ﬁnishing mill to compensate the ﬂatness change during the cooling stage. This measurement has the advantages of low investment and easy implementation, compared with the methods mentioned before for realizing uniform cooling. This shape compensation control strategy has been employed to improve the strip shape quality in the actual production. The aim ﬂatness values at the exit of ﬁnishing mill are setup to be 1020 I Unit according to the strip material and the gauge. To make a clear about the control effect of the slight center wave rolling strategy, comparison work has been done through tracking the ﬂatness qualities of a large amount of strips. In ﬂatness control model, aim ﬂatness values of 10 or 20 I Unit were setup for some strips, while 0 I Unit was setup for others. Firstly, the ﬂatness at the exit of ﬁnishing mill was measured by the ﬂatness gauge meter, and then the actual ﬂatness of that strip was measured during the uncoiling process. Part of the tracking results is listed in Table. 4. All strips rolled to be center buckles have good ﬂatness qualities after cooling. On the contrary, those rolled to be ﬂat become wavy edges after the cooling, and even severer for those rolled to be wavy edges. In turn, it can be deduced that the compensation control strategy of slight central wave rolling has a good effect. 5. Conclusions A thermal, microstructural and mechanical coupling analysis model for predicting ﬂatness change of the steel strip during the run-out table cooling was established using ABAQUS Finite Element Software in this work. (1) Esaka phase transformation kinetics model was employed to calculate the phase transformation happened during the cooling process of hot rolled strip, and coupled with temperature calculation using the user subroutine program HETVAL. (2) The elasto-plasticity constitutive model of the steel material including thermal and microstructural behaviors at the same time, in which the conventional elastic and plastic strains, thermal strain, phase transformation strain resulted by phase volume change and transformation induced plastic strain calculated using Greenwood-Johnson model modiﬁed by Leblond were taken into account, was employed and realized using the user subroutine program UMAT. (3) The conclusion that the ﬂatness of steel strip will develop to edge wave under the functions of the transverse thermal and microstructural behavior differences during the run-out table cooling procedure was acquired through the analysis results of this model. Calculation results of this analysis model agree well with the actual measurements. (4) It is veriﬁed that the phase transformation has an important inﬂuence on prediction accuracy of the residual stress generation and the effect of transformation induced plasticity should not be neglected for precision analysis on the deformation of the steel plate during the cooling. (5) The strip shape compensation control strategy of slight center wave rolling was proposed on the basic of analysis results of this model and applied in the actual production with a good effect. X. Wang et al. / Applied Mathematical Modelling 37 (2013) 586–609 609 References [1] J. Hidveghy, J. Michel, M. Bursak, Residual stress in microalloyed steel sheet, Metalurgija 42 (2) (2003) 103–106. [2] M.M. Prieto, L.S. Ruíz, J.A. Menèndez, Thermal performance of numerical model of hot strip mill runout table, Ironmaking Steelmaking 28 (6) (2001) 474–480. [3] Zhengdong Liu, Experiments and mathematical modeling of controlled runout table cooling in a hot rolling mill, Ph.D Dissertation, The University of British Columbia, 2001. [4] C.G. Sun, H.N. Han, J.K. Lee, Y.S. Jin, S.M. Hwang, A ﬁnite element model for the prediction of thermal and metallurgical behavior of strip on run-outtable in hot rolling, ISIJ Int. 42 (4) (2002) 392–400. [5] S. Serajzadeh, Prediction of temperature distribution and phase transformation on the run-out table in the process of hot strip rolling, Appl. Math. Model. 27 (2) (2003) 861–875. [6] H. Yoshida, Analysis of ﬂatness of hot rolled steel strip after cooling, Transactions ISIJ 24 (3) (1984) 212–220. [7] Wang. Shyi-Chin, Chiu. Fon-Jen, Ho. Tsan-Ying, Characteristics and prevention of thermomechanical controlled process plate deﬂection resulting from uneven cooling, Mater. Sci. Technol. 12 (1) (1996) 64–71. [8] H. Yoshida, T. Tamari, T. Ito, An analysis of temperature, thermal stress and shape defect during accelerated cooling in steel plates, Tetsu-to-Hagane (Journal of the Iron and Steel Institute of Japan) (Japan), 83(2) (1997) 121–126. [9] T.Suzuki, K. Isaka, Control of the residual stress of plates, in: Proceedings of the 7th International Conference on Steel Rolling (Steel Rolling ‘98), Chiba, Japan, The Iron and Steel Institute of Japan, 1998, pp. 601–605. [10] T. Tani, K. Ohe, T. Ueda, H. Fujiuchi, T. Tada, Y. Tsutsumi, Development of an on-line shape control system of TMCP steel plate, in: Proceedings of The 7th International Conference on Steel Rolling (Steel Rolling ‘98), Chiba, Japan, The Iron and Steel Institute of Japan, 1998, pp. 589–594. [11] Zh. Cai, Research on buckling behavior of hot-rolled strip after cooling, Ph.D Dissertation, Northeast University, vol. 6, 1998, (in Chinese). [12] H.N. Han, J.K. Lee, H.J. Kim, Young-Sool Jin, A model for deformation, temperature and phase transformation behavior of steels on run-out table in hot strip mill, J. Mater. Process. Technol. 128 (2002) 216–225. [13] R. Colás, L.A. Leduc, M.A. Neri, Prediction of shape defects during cooling of hot rolled low carbon steel strip, Ironmaking Steelmaking 31 (1) (2004) 93– 96. [14] Zh. Zhou, Peter F. Thomson, YeeCheong Lam, Daniel D.W. Yuen, Numerical analysis of residual stress in hot-rolled steel strip on the run-out table, J. Mater. Process. Technol. 132 (2003) 184–197. [15] H. Ogai, M. Ito, R. Hirayama, Consistent shape prediction simulator after hot rolling mill, Nippon Steel Technical Report, January 89 (2004) 43–49. [16] Zh. Zhou, YeeCheong Lam, P.F. Thomson, D.D.W. Yuen, Numerical analysis of the ﬂatness of thin, rolled steel strip on the runout table, in: Proceedings of the Institution of Mechanical Engineers, Part B: Journal of Engineering Manufacture, 2007, 221(2), pp. 241–254. [17] E. Nikitenko, B.C. Gris, A mechanism of post-rolling deterioration in hot band ﬂatness during coiling, Iron Steel Technol. 6 (10) (2009) 60–63. [18] J.M. Koo, S.R. Ryoo, Ch.S. Lee, Ch.G. Sun, H.N. Han, S.M. Hwang, Prediction of residual stresses in a plate subject to accelerated cooling – a 3-D ﬁnite element model and an approximate model, ISIJ Int. 47 (8) (2007) 1149–1158. [19] S. Sjöström, Interactions and constitutive models for calculating quench stresses in steel, Mater. Sci. Technol. 1 (10) (1985) 823–829. [20] R.V. Fryan, The inﬂuence of material uniformity on the heat treat distortion of a steel ring, Dissertation for Ph.D, Case Western Reserve University, January, 1995. [21] X. Chen, Computer simulation of the thermal mechanics of steel quenching, Dissertation for Ph.D, The Oregon Graduate Institute of Science and Technology, April, 1998. [22] F.D. Fischer, G. Reisner, E. Werner, K. Tanaka, G. Cailletaud, T. Antretter, A new view on transformation induced plasticity (TRIP), Int. J. Plast. 16 (2000) 723–748. [23] P.M.C.L. Pacheco, M.A. Savi, A.F. Camarão, Analysis of residual stresses generated by progressive induction hardening of steel cylinders, J. Strain Analysis 36 (5) (2001) 507–517. [24] X. Yao, L.H. Zhu, M. Victor Li, Finite element analysis of residual stress and distortion in an eccentric ring induced by quenching, in: Transactions of Materials and Heat Treatment Proceedings of the 14th IFHTSE Congress, 2004, 25(5), pp. 746–751. [25] E.P. Silva, P.M.C.L. Pacheco, M.A. Savi, Finite element analysis of the phase transformation effect in residual stresses generated by quenching in notched steel cylinders, J. Strain Analysis 40 (2) (2005) 151–160. [26] S. Casotto, F. Pascon, A.M. Habraken, S. Bruschi, Thermo-mechanical-metallurgical model to predict geometrical distortions of rings during cooling phase after ring rolling operations, Int. J. Mach. Tools Manuf 45 (2005) 657–664. [27] X.D. Wang, Q. Yang, A.R. He, Calculation of thermal stress affecting strip ﬂatness change during run-out table cooling in hot steel strip rolling, J. Mater. Process. Technol. 207 (2008) 130–146. [28] O. Kwon, A technology for prediction and control of microstructural changes and mechanical properties in steel, ISIJ Int. 32 (3) (1992) 350–358. [29] L. Taleb, F. Sidoro, A micromechanical modeling of the Greenwood-Johnson mechanism in transformation induced plasticity, Int. J. Plast 19 (2003) 1821–1842. [30] ABAQUS Standard Version 6.5, User Manual, Theory Manual, Hibbitt, Karlsson & Sorensen, Inc. 2005. [31] M. Becker, C. Jordan, S.K. Lachhander, A. Mengel, M. Renauld, Prediction and measurement of phase transformations, phase-dependent properties and residual stresses in steels, in: Proceedings of the 7th International Conference on Trends in Welding Research, May 16–20, 2005, Callaway Gardens Resort, Pine Mountain, Georgia, USA, 1007–1012. [32] S.D. Cox, S.J. Hardy, D.J. Parker, Inﬂuence of runout table operation setup on hot strip quality, subject to initial strip condition: heat transfer issues, Ironmaking Steelmaking 28 (5) (2001) 363–372. [33] M.C. Zhang, J.X. Dong, Y.P. Zeng, Y. Sun, Zh.M. Yang, Dynamical microstructure evolution of Q235 low carbon steel during high temperature deformation. Journal of University of Science and Technology Beijing, 2005, 27(2), 183–186 (in Chinese). [34] S. Peregrina, Redondo JM. García, Quiroga P. Fdz, García D. Glz, D. García, Hot strip ﬂatness optimization by means of edge masking in the ROT, in: This paper was presented at the Steel Rolling 2006 9th International & 4th European Conferences from 19–21 June, 2006, which was organised by ATS (Association Technique de la Siderurgie Française), Session. 1, 2–9.